Magneto-resistance in a lithography defined single constrained domain wall
Yudong Wang,1 C.H. de Groot,1, a) D. Claudio-Gonzalez,2 and Hans Fangohr3
1)School of Electronics and Computer Science University of Southampton SO17 1BJ,
2)Division of Engineering Campus Irapuato-Salamanca, Department of Multidisciplinary Studies,
University of Guanajuato, C.P. 38940, Yuriria, Mexico
3)School of Engineering Science University of Southampton SO17 1BJ, United Kingdom
(Dated: 5 November 2010)
We have successfully measured domain wall magnetoresistance in a single lithographically constrained domain
wall. A H-shaped Ni nano-bridge was fabricated by e-beam lithography with the two sides being single mag-
netic domains showing independent magnetic switching and the connection between the sides constraining the
domain wall when the sides line up anti-parallel. The magneto-resistance curve clearly identifies the magnetic
configurations that are expected from a spin valve-like structure. The value of the magneto-resistance at room
temperature is around 0.1% or 0.4 Ω. This value is shown to be in agreement with a theoretical formulation
based on spin accumulation. Micromagnetic simulations show it is possible to reduce the size of the domain
wall further by shortening the length of the bridge.
Keywords: Spin-valve, Single constrained domain wall, Domain wall magnetoresistance, DWMR
The research of spin-based logic will not only benefit
the understanding of physics but also give possibility to
fabricate faster and denser memory devices1,2. Domain
wall magneto-resistance (DWMR) occurs when electrons
travel from one side of the magnetic domain wall to
another non-adiabatically. The DWMR is reported
in many different structures such as ring structure3–6,
line structure7–12, atom-contact structure13,14, zigzag
structure15,16and bridge structure17,18.In line-shape de-
vices, the magneto-resistance effect of the domain wall
is relatively small because the classic resistance of the
line hides the DWMR effect. In the point connect-
ing structure the magnetoresistance can be very large
due to the ballistic transport of the electrons, but
the fabrication procedures such as mechanical break
junctions19,electrical break junctions20 and electrochem-
ical junctions21 are not suitable for the industrial
fabrications22, and the measurements are subject to
In 1999, Bruno24 proposed that in nano-structured de-
vices the domain wall width can be constricted by geo-
metric means. A sudden large expansion of the magnetic
area will constrict the domain wall as the cost of increas-
ing the area of the domain wall outweighs the exchange
interaction. In this letter we report the experimental
realisation of this proposed structure and show magneto-
resistance in a lithographically defined constrain domain
wall structure in between two independently switching
single magnetic domains. This is the first in-plane trans-
port measurement of an individual magnetic structure
completely at the nano-scale using standard methods.
a)Electronic mail: [email protected]
FIG. 1. SEM micrograph of the Ni domain wall structure with
the Au contact lines. The bridge length 2d0 = 94.4 nm and
width s0 = 45.6 nm. The left domain whose size is 100× 400
nm can be seen as a pinned pad of the spin-valve, and the
right domain 200× 400 nm is a switchable pad.
The device was fabricated on a Si p-type < 100 > wafer
with 17-33 Ωcm resistivity. A 50nm-thick SiO2 layer was
thermally grown on the front side of the wafer. Two lay-
ers of Au were deposited by photo lithography and metal
lift-off. The thickness of the first gold layer was 22nm
allowing the contact the e-beam defined layers later on,
while the second layer was 200 nm to allow probing. The
third layer of Au wires which was 22 nm-thick and 200
nm-wide were patterned by a JEOL e-beam lithography
system on PMMA and Copolymer bi-layer e-beam re-
sist. The Au deposition was done at pressure 5 × 10−6
FIG. 2. SEM micrograph showing top view of the whole de-
vice structure including four-point probe measurement set up
and insert showing cross section view. The ordered number in
cross section shows the fabrication sequence. The pads num-
bered 1-4 indicate the probes’ connection during our measure-
ment Rdev = V14/I23.
mbar and deposition rate 1 Å/s. The lift-off was done
in N-Methyl-2-pyrrolidone (NMP) for 30 mins at room
temperature. The 20 nm-thick Ni nano-structure was
build in the fourth metal layer. The Ni deposition had
the same condition as the Au deposition except for the
deposition rate, which was 0.5 Å/s. Fig. 1 shows the Ni
nano-bridge together with the e-beam defined Au layer.
The critical alignment between the two layers shows an
alignment tolerance of better than 20 nm.
The Au structure allows a four point measurement
technique to be employed in the measurement of the do-
main wall structure such that only the Ni structure con-
tributes to the resistance as shown in Fig. 2. Room
temperature MR measurement were performed with a
Lakeshore EMTTP4 magnetic probe station and an Ag-
ilent B1500 semiconductor parameter analyser.
III. RESULT AND DISCUSSION
Fig. 3 shows the room temperature magneto-resistance
effect of the nano-bridge. The resistance-field pattern
shows the typical step-like behaviour of a spin-valve like
MR structure in which both sides switch independently.
The high coercive side (100× 400 nm2 domain; left side
in Fig. 1) switches at around 25mT and the low coer-
cive side (200 × 400 nm2 domain) switches near 5 mT.
These experimental values are slightly smaller than those
derived from an OOMMF25 simulation as shown in Fig.
4. Nevertheless, a clear plateau is identified in the MR
curve in which the domains are anti-parallel leading to a
domain wall in the nano-bridge and hence domain wall
magneto-resistance of around 0.1% or 0.4 Ω which is sim-
ilar to the result in Ni necked wires reported by Lepadatu
FIG. 3. Room temperature magneto-resistance curves of the
Ni nano-bridge. The blue curve shows the device resistance
when increasing magnetic field, while the green curve shows
the decreasing field. Data are averaged over 6 individual mea-
FIG. 4. OOMMF25 magnetization - magnetic field hysteresis
loops. The model’s geometrical size is based on the fabricated
device shown in Fig. 1. The simulation parameters for Ni,
exchange stiffness A = 9×10−12 J/m, and saturation magne-
tization Ms = 490kA/m are used. The curve shows both the
parallel and anti-parallel states of our device.
and Xu in 200426.
Ieda et al.27 provided an equation to explain the
DWMR effect based on spin accumulation:
∆R = 2P 2ρ0λFA
−1F (ξ) (1)
where P is the polarization of the conduction spin, ρ0 is
the classic resistivity, λF is the spin diffusion length, A is
the cross sectional area of the constriction, and F (ξ) is a
function of the ratio w/λF in which w is the domain wall
width. The reduction on the domain width will increase
the F (ξ)’s value27.
We have previously shown28 using a micromagnetic
simulation that the the domain wall width can be re-
duced by scaling the geometrical size of the bridge either
FIG. 5. OOMMF micromagnetic simulation results showing
the constrained domain wall length as a function of 2d0 for
fixed ratio s0/s1 = 0.10. Squares are simulated values. A line
is guide to the eye. The star indicates the experimental point.
through a reduction of the s0/s1 ratio or through limit-
ing the bridge length 2d0. Using the experimental ratio
of s0/s1 = 0.10, we can calculate the value of the do-
main wall width once demagnetisation effects are taken
into account. The calculations as displayed in Fig.5 show
that our current value of the domain wall width is 42nm.
Entering this value in to the Equation 1 together with a
spin polarization of P = 20%, λF = 21 nm and ρ0 = 520
nΩm18 we arrive at a value of ∆R = 0.402 Ω which is
close to our measurement result. Further reduction of
the length of the bridge will significantly enhance the
We have successfully measured domain wall magne-
toresistance in a single lithographically constrained do-
main wall. The value of the magneto-resistance at room
temperature is around 0.1% or 0.4 Ω in agreement with a
theoretical formulation based on spin accumulation. Mi-
cromagnetic simulations show it is possible to reduce the
size of the domain wall further by shortening the length
of the bridge allowing larger MR and a quantitative test
of the effect of a reduction of the domain wall on the
We would like to thank Dr Martin Charlton for e-beam
training, Dr Khaled Husain for advise on lithography,
and Prof. Mike Gibbs for discussions on magnetic be-
1B. Behin-Aein, D. Datta, S. Salahuddin, and S. Datta, Nature
Nanotechnology online (2010), 10.1038/nnano.2010.31.
2D. A. Allwood, G. Xiong, C. C. Faulkner, D. Atkinson, D. Petit,
and R. P. Cowburn, Science 309, 1688 (2005).
3M. Kläui, C. A. F. Vaz, J. Rothman, J. A. C. Bland, W. Werns-
dorfer, G. Faini, and E. Cambril, Physical Review Letters 90,
4C. C. Chen, C. C. Chang, Y. C. Chang, C. T. Chao, C. Y. Kuo,
L. Horng, J. C. Wu, T. Wu, G. Chern, C. Y. Huang, M. Tsun-
oda, and M. Takahashi, IEEE Transactions on Magnetics 43,
5C. Yu, S. F. Lee, Y. D. Yao, M. S. Wong, E. W. Huang, Y. R.
Ma, J. L. Tsai, and C. R. Chang, Physica B 327, 247 (2003).
6M.-F. Lai, Z.-H. Wei, C.-R. Chang, J. C. Wu, J. H. Kuo, and
J.-Y. Lai, Physical Review B 67, 104419 (2003).